# Theoretical approach to determine dynamic fatigue strength characteristics of ceramics under variable loading rates on the basis of SCG concept

- 29 Downloads

## Abstract

This paper presents a theoretical approach to determine the dynamic fatigue strength characteristics of ceramics under variable loading rates on the basis of the slow crack growth (SCG) concept. First, a probabilistic effective inert strength model was derived on the basis of the SCG concept in conjunction with the Weibull distribution for ceramics subjected to multi-stage loading. Second, a four-point bending test was conducted on \(\hbox {Al}_{{2}}\hbox {O}_{{3}}\) under constant and two-stage variable loading rates, and the fracture surface was then observed. The experimental data that depend on loading rates can be unifiedly evaluated after converting the data to the effective inert strength, obeying the three-parameter Weibull distribution. In addition, the Weibull plots of the inert strength, which were calculated from the inclusion size on the fracture surface using the grain fracture model, showed good agreement with the three-parameter Weibull distribution for the converted effective inert strength. These analytical results theoretically indicate that dynamic fatigue under variable loading rates occurs by obeying SCG at the inclusion. Further, the inert strength and its scatter depend on the size and distribution of inclusions.

## Keywords

Ceramics Variable loading rate Dynamic fatigue strength SCG Inclusion size Inert strength## Notes

### Acknowledgements

I would like to show my greatest appreciation to Prof. K. Ogi (Ehime University, Japan) whose comments and advice were highly valuable throughout the course of my study.

### Funding

This work was supported by JSPS KAKENHI [Grant Number 17K14563].

## References

- Breder K (1995) Time-dependent strength degradation of a siliconized silicon carbide determined by dynamic fatigue. J Am Ceram Soc 78(10):2680–2684CrossRefGoogle Scholar
- Choi G, Horibe S (1993) The influence of variable-amplitude loading on cyclic-fatigue crack growth in silicon nitride. J Mater Sci Lett 12(24):1886–1887CrossRefGoogle Scholar
- Choi SR, Nemeth NN, Gyekenyesi JP (2005) Exponential slow crack growth of glass and advanced ceramics-dynamic fatigue. Fatigue Fract Eng Mater Struct 28(5):489–497CrossRefGoogle Scholar
- Evans AG (1980) Fatigue in ceramics. Int J Fract 16(6):485–498CrossRefGoogle Scholar
- Evans AG, Fuller ER (1974) Crack propagation in ceramic materials under cyclic loading conditions. Metall Trans 5:27–33Google Scholar
- Evans AG, Johnson H (1975) The fracture stress and its dependence on slow crack growth. J Mater Sci 10(2):214–222CrossRefGoogle Scholar
- Evans AG, Lange FF (1975) Crack propagation and fracture in silicon carbide. J Mater Sci 10(10):1659–1664CrossRefGoogle Scholar
- Evans AG, Wiederhorn SM (1974a) Proof testing of ceramic materials-an analytical basis for failure prediction. Int J Fract 10(3):379–392CrossRefGoogle Scholar
- Evans AG, Wiederhorn SM (1974b) Crack propagation and failure prediction in silicon nitride at elevated temperature. J Mater Sci 9(2):270–278CrossRefGoogle Scholar
- Evans AG, Russell LR, Richerson DW (1975) Slow crack growth in ceramic materials at elevated temperatures. Metall Mater Trans A 6:707–716CrossRefGoogle Scholar
- Gilberta CJ, Ritchiea RO (1998) Transient fatigue-crack growth behavior following variable-amplitude loading in a monolithic silicon nitride ceramic. Eng Fract Mech 60(3):303–313CrossRefGoogle Scholar
- Guiu F, Reece MJ, Vaughan DAJ (1991) Cyclic fatigue of ceramics. J Mater Sci 26:3275–3286CrossRefGoogle Scholar
- Hasselman DPH, Chen EP, Ammann CL, Doherty JE, Nessler CG (1975) Failure prediction of the thermal fatigue of silicon nitride. J Am Ceram Soc 58(11–12):513–516CrossRefGoogle Scholar
- Hoshide T, Hiramatsu H (1999) A microstructural approach to flaw size dependence of strength in engineering ceramics. Fatig Fract Eng Mater Struct 22(12):1029–1039CrossRefGoogle Scholar
- Hoshide T, Ohara T, Yamada T (1988) Fatigue behavior of ceramic materials under variable stress amplitude. Eng Fract Mech 31(2):339–347CrossRefGoogle Scholar
- Kamiya N, Kamigaito O (1982) Thermal fatigue life of ceramics under mechanical load. J Mater Sci 17(11):3149–3157CrossRefGoogle Scholar
- Matsuda S (2016) Fracture characteristics of silicon nitride ceramic ball subjected to thermal shock. J Mater Sci 51(11):5502–5513CrossRefGoogle Scholar
- Matsuda S, Ogi K (2017) Effect analysis of loading rate on relationship between strength and flaw size of ceramics using probabilistic model on the basis of SCG concept. Trans JSME 83(847):16–00369Google Scholar
- Matsuda S, Watanabe R (2011) Estimation of dynamic fatigue strengths in brittle materials under a wide range of stress rates. J Mater Sci 46(15):5056–5063CrossRefGoogle Scholar
- Ogi K, Ito K (2011) A probabilistic approach for thermal shock fatigue life of glass. Fatigue Fract Eng Mater Struct 34(9):643–653CrossRefGoogle Scholar
- Ogi K, Yashiro S, Niimi K (2010) A probabilistic approach for transverse crack evolution in a composite laminate under variable amplitude cyclic loading. Compos A 41(3):383–390CrossRefGoogle Scholar
- Okabe N, Ikeda T (1991) Strength evaluation method and design optimization for ceramic gas turbine blades. Mater Sci Eng A 143(1–2):11–19CrossRefGoogle Scholar
- Pan LS, Matsuzawa M, Horibe S (1998) Stress rate dependence of fracture strength in pre-cracked zirconia ceramics. Mater Sci Eng A 244(2):199–206CrossRefGoogle Scholar
- Pfingsten T, Glien K (2006) Statistical analysis of slow crack growth experiments. J Eur Ceram Soc 26(15):3061–3065CrossRefGoogle Scholar
- Phani KK (1988) Analysis of static and dynamic fatigue of polycrystalline alumina. J Mater Sci 23(11):3864–3868CrossRefGoogle Scholar
- Quinn GD, Salem J, Bar-on I, Cho K, Foley M, Fang H (1992) Fracture toughness of advanced ceramics at room temperature. J Res Natl Inst Stand Technol 97(5):579–607CrossRefGoogle Scholar
- Ritter JE (1995) Predicting lifetimes of materials and material structures. Dent Mater 11(2):142–146CrossRefGoogle Scholar
- Ritter JE Jr, Humenik JN (1979) Static and dynamic fatigue of polycrystalline alumina. J Mater Sci 14(3):626–632CrossRefGoogle Scholar
- Sakai T, Tanaka T (1980) Estimation of three parameters of Weibull distribution in relation to parameter estimation of fatigue life distribution: continued report. J Soc Mater Sci Jpn 29(316):17–23CrossRefGoogle Scholar
- Seshadri SG, Srinivasan M, Weber GW (1982) Evaluation of slow crack growth parameters for silicon carbide ceramics. J Mater Sci 17(5):1297–1302CrossRefGoogle Scholar
- Siegmund T (2004) A numerical study of transient fatigue crack growth by use of an irreversible cohesive zone model. Int J Fatigue 26(9):929–939CrossRefGoogle Scholar
- Tanaka T, Nakayama H, Okabe N, Yamamoto S, Fukui S (2002) Creep rupture map of engineering fine ceramics. In: Bradt RC et al (eds) Fracture mechanics of ceramics, vol 10. Plenum Press, New York, pp II-308–II-326Google Scholar
- Teixeira EC, Piascik JR, Stoner BR, Thompson JY (2007) Dynamic fatigue and strength characterization of three ceramic materials. J Mater Sci Mater M 18(6):1219–1224CrossRefGoogle Scholar
- To T, Célarié F, Roux-Langlois C, Bazin A, Gueguen Y, Orain H, Le Fur M, Burgaud V, Rouxel T (2018) Fracture toughness, fracture energy and slow crack growth of glass as investigated by the single-edge precracked beam (SEPB) and chevron-notched beam (CNB) methods. Acta Mater 146:1–11CrossRefGoogle Scholar
- Usami S, Kimoto H, Takahashi I, Shida S (1986) Strength of ceramic materials containing small flaws. Eng Fract Mech 23(4):745–761CrossRefGoogle Scholar
- Wiederhorn SW, Bolz LH (1970) Stress corrosion and static fatigue of glass. J Am Ceram Soc 53(10):543–548CrossRefGoogle Scholar
- Zhu P, Lin Z, Chen G, Ikeda K (2004) The predictions and applications of fatigue lifetime in alumina and zirconia ceramics. Int J Fatigue 26(10):1109–1114CrossRefGoogle Scholar